*203*
*59*
*3MB*

*English*
*Pages [151]*
*Year 1966*

*Table of contents : Front CoverTitle PageTranslation Editor’s ForewordPrefaceContents1. Introduction2. Impurity Levels and Impurity Bands3. Neutralization in Terms of Impurity Configurations . Crystal Momentum4. SCREENING5. Characteristics o f a Many-Electron System6. Equations for Green Functions7. Perturbation Theory: Summary of Results8. Semiclassical Approximation9. Density of States10. The Fermi Level in a Heavily Doped Semiconductor11. The Momentum Distribution Function For T = 0 and a Screened Potential12. Static Electrical Conductivity13. Absorption of Electromagnetic Waves in a Heavily Doped Homopolar Semiconductor14. Heavily Doped Semiconductor with an Incompletely Homopolar Lattice15. Contact o f Two Heavily Doped SemiconductorsReferencesIndex*

V.L. Bonch-Bruyevich

THE ELECTRONIC THEORY OF HEAVILYDOPED SEMICONDUCTORS

T H E E L E C T R O N IC T H E O R Y O F H E A V IL Y D O P E D SE M IC O N D U C T O R S

Originally published by the Academy of Sciences of the USSR as: VOPROSY ELEKTRONNOY T E O R II SI i /

n

O LEGIROVAN NYKH POLUPROVODNIKOV

MOSCOW 1965

T H E E L E C T R O N IC T H E O R Y O F H E A V IL Y D O P E D SE M IC O N D U C T O R S BY

V. L. BONCH-BRUYEVICH ni

Moscow State University

Translated by Scripta Technica, Inc.

Translation Editor: Robert S. Knox Department of Physics and Astronomy University of Rochester

NEW YORK

AMERICAN ELSEVIER PUBLISHING COMPANY INC. 1966

SOLE DISTRIBUTORS FO R G REAT B R ITA IN

ELSEVIER PUBLISHING COMPANY, LTD.

Barking, Essex, England

SOLE DISTRIBUTORS FO R T H E C O N T IN E N T O F E U R O PE

ELSEVIER PUBLISHING COMPANY

Amsterdam, The Netherlands

Library of Congress Catalog Card Number: 66-25115

CO PYRIG HT ©

1966

BY A M E R IC A N E LSEV IE R P U B L ISH IN G C O M PA N Y , IN C .

A L L RIGHTS RESERVED. T H IS BOOK OR ANY P A R T T H E R E O F M U ST N O T BE REPRODUCED IN ANY F O R M W IT H O U T T H E W R IT T E N P E R M IS S IO N O F T H E P U B L IS H E R , A M E R IC A N E LSEV IE R PU B L ISH IN G C O M P A N Y , IN C .,

52

V A N D ERB ILT A V E N U E, N E W YORK, N . Y.

M A N U FA C TU R ED IN T H E U N ITE D STATES O F A M ER IC A

10017

T r a n s l a t i o n E d i t o r ’s F o r e w o r d

The techniques of many-body theory are best known in their application to the electronic states of metals and to statistical problems. In the theory of heavily doped semiconductors both the quantum and statistical mechanical aspects of the problem are prominent. The present tract is a review by Professor Bonch-Bruyevich, one of Russia’s leading solid state theorists, of the quantitative progress which has been made in this chal lenging field. The English edition is a translation of the Soviet original which appeared in 1965 and should be of value as a reference to all physicists working in this field. R. S. ROCHESTER,

N. Y . ,

MAY 1 9 6 6

V

KNOX

Preface

The current interest in solid state theory is, in the main, the result of confluence of two factors: recent progress in the problem of many bodies in quantum-statistical mechanics, and demands of practical semiconductor physics occasioned, in turn, by the ever increasing use of solid state devices in sci ence and technology. Professor Bonch-Bruyevich has rendered a real and welltimed service in pulling together the available information on heavily doped semiconductors, because the problems associated with these materials are among the most pressing in modern applied and theoretical physics. The reader will find here a detailed review of the many-electron approach to the theory of doped semiconductors, as well as a systematic exposition of the many studies done in this area (much of it by the author and his students). Some of the interesting topics covered are the energy spectrum of heavily doped semiconductors, pulse dis tributions in them, as well as screening effects and absorption of electromagnetic waves. The necessary mathematical ma chinery of the theory is explained simply and concisely. It is hoped that the book will prove of value not only to specialists in the field, but also to a wider group of solid-state theoreticians and experimentalists. S. T Y A B L IK O V

Contents TRANSLATION EDITOR’S FOREWORD

v

PREFACE

vii

1. INTRODUCTION

1

2. IMPURITY LEVELS AND IMPURITY BANDS

5

3. NEUTRALIZATION IN TERMS OF IMPURITY CONFIGURA TIONS. CRYSTAL MOMENTUM

]]

4. SCREENING

15

5. CHARACTERISTICS OF A MANY-ELECTRON SYSTEM

19

6. EQUATIONS FOR GREEN FUNCTIONS

33

7. PERTURBATION THEORY: SUMMARY OF RESULTS

45

8. SEMICLASSICAL APPROXIMATION

57

9. DENSITY OF STATES

65

10. FERMI LEVEL IN A HEAVILY DOPED SEMICONDUCTOR

77

11. MOMENTUM DISTRIBUTION FUNCTION FOR A SCREENED POTENTIAL

81

T = 0 AND

12. STATIC ELECTRICAL CONDUCTIVITY

89

13. ABSORPTION OF ELECTROMAGNETIC WAVES IN A HEAVILY DOPED IIOMOPOLAR SEMICONDUCTOR

97

14. HEAVILY DOPED SEMICONDUCTOR WITH AN INCOMPLET E LY IIOMOPOLAR LATTICE

113

15. CONTACT OF TWO HEAVILY DOPED SEMICONDUCTORS

117

REFERENCES

125

INDEX

'

129 IX

CHAPTER 1

Introduction

The study of the electronic properties of semiconductors containing a rather large amount of impurity has become extremely important in recent years.* This is primarily as sociated with the discovery of tunnel diodes (see, for example, the review [1]); however, the area of application of heavily doped m aterials is actually much broader. These semiconductors are used in, among other things, lasers and thermoelectric devices, semiconductor catalysts and, of course, thin films. The term “ impurity” is not necessarily to be interpreted literally—it can refer to any structural point defects that lead to a disturbance of strict periodicity of the lattice. Disordered alloys (including metallic m aterials) represent the limiting case of m aterials of the type under consideration.** Obviously the study of heavily doped semiconductors is a part of the more general problem of disordered structures. The study of the latter is of nearly prim ary interest in present-day solid state physics. The phonon [2-5] and electron [6] spectra of m aterials of this type have been studied for the case of relatively low im purity concentration. The method employed in the works cited represents, in essence, a reasonable perturbation theory based *The exact meaning of the expressions “rather a large amount of impurity,” “heavily doped semiconductor,” etc., will be explained later. **In essen ce, any impure specimen (the only thing semiconductor physics dealt with in its early stages of development) is heavily doped. However, serious research was begun only after it became possible to obtain materials doped with a specific impurity and at a specific concentration.

1

2

ELECTRON THEORY OF SEM ICONDUCTORS

on the expansion of certain quantities in a series in powers of the impurity concentration. One or another of the characteristics of an ideal crystal, assumed to be known, is taken as the zeroorder approximation. In this fashion it has been possible to ex plain a number of the important properties of slightly disordered systems and to obtain a quantitative description of their energy eigenvalue spectra. However, in the case of the electron spectra the conditions for the applicability of the series expansions are somewhat more restrictive than one would like for consideration of most m aterials of experimental interest. Thus itwill be seen later that in the semiconductors employed in tunnel diodes and lasers (Ge, GaAs, InSb) the impurity concentration is greater than that required for use of the expansions. In this instance the doping element is more of a microimpurity so that a statement of the problem based on the specific properties of the correspond ing ideal crystal makes complete sense. Moreover, some specific effects that require special study also appear. These effects will be examined in the next three sections; a definition of the con cept of a “heavily doped semiconductor” will also be given. Later (Chaps. 5, 6) a mathematical device suitable for de scribing the systems of interest to us will be considered. Within the lim its of the present review only a discussion of the type mentioned above will be given; a more detailed knowledge of the device can be obtained from the papers cited in the appropriate chapters. The reader who is interested only in the results of the theory can omit Chap. 6, as well as all the subsequent mathe matical portions, limiting himself only to the summaries of the results located at the end of Chaps. 7, 9-15. Chapters 7-11 and Chap. 14 are devoted to a study of the energy spectrum of heavily doped semiconductors and the associated problems. Some prob lems in kinetics which are important for an interpretation of many of the experimental data are considered in Chaps. 12, 13. Finally, in Chap. 15 the characteristics of intrinsically inhomo geneous system s—the contact region of two heavily doped semi conductors with identical or different types of conductivity—are investigated. It should be noted that the theory of heavily doped semicon ductors in its complete form started to evolve quite recently and many important problems have yet to be solved. Thus, for example, galvanomagnetic effects have not been completely in vestigated from a theoretical point of view. Explicit equations have recently been derived for the Hall and thermoelectric power constants of a heavily doped semiconductor [118], The corrections to the equations of the standard theory are small in the limiting case of heavy doping.

INTRODUCTION

3

Some of the usual concepts of semiconductor physics, used consistently for interpreting experimental data, are inadequate for the problem in heavily doped m aterials and sometimes simply become meaningless. The need to call this circumstance to the attention of research ers, as well as the desire to draw the at tention of theorists to the complex and interesting problems of disordered system s, served as the prim ary reason for compil ing the present review.

CHAPTER 2

I m p u r i t y L e v e ls and I m p u r it y B a n d s

It is simpler to approach the definition of a “ heavily doped semiconductor” by considering the change in the band spectrum of the crystal as the impurity concentration increases. It is well known that isolated impurity atoms can lead to the creation of discrete levels located in the forbidden band. The wave func tion of an electron occupying such a level is localized in the vicinity of the impurity atom. The energy spectrum of the semiconductor in this case of “light doping” is represented schematically in Fig. 1 (the “ allowed” regions of the continuous spectrum are crosshatched). For definiteness let us assume that each impurity atom gives rise to only one discrete level. The symbols are the usual ones: Ee —the bottom of the conduction

Fig. 1. Lightly doped semi conductor.

5

6

ELECTRON THEORY OF SEMICONDUCTORS

band, Ev —the top of the valence (i.e., the bottom of the forbidden) band, E t —impurity level. Obviously the concept of impurity atoms isolated from each other can be valid only as long as the “ regions of localization” of the associated electrons do not overlap to an appreciable extent. (For this to be true the im purity concentration n must be quite small.) When such over lapping sets in, the impurity levels should “ spread” in the same way as do the levels of the atoms of a crystal relative to their discrete nature in the vapor phase.* A complete band of allowed states (separated, however, from the conduction band by a forbidden region) appears in the for bidden band. It is commonly called the impurity band although it must be admitted that this is an unfortunate designation: nothing is said here concerning the dependence of the energy on crystal momentum. Moreover, using the concept of crystal momentum here requires justification because, generally speak ing, the impurity atoms are not periodically arranged. Con versely, it is more reasonable to assume that their arrangement in the lattice is random. In a macroscopically homogeneous crystal the average impurity concentration is, of course, con stant over a relatively large region; however, in small volumes (for example, in a sphere with a radius of the order of the radius of the effective interatomic force) the variation in concentration can be considerable. This circumstance leads to a second mechanism for the “ spreading” of levels. That is, we isolate some arbitrary impurity atom and consider the effect of all the other impurity atoms on the electron localized near it. A vari ation of concentration as we consider different arbitrary atoms obviously leads to a variation in the potential energy of the as sociated electrons, i.e., ultimately to a spread in the ionization energy. This may be detected, sometimes optically, as a broadening of the level. To differentiate it from the first (“ quasi chemical” ) mechanism for the development of an impurity band, this second mechanism can be called the “van der Waals” mechanism. We will designate as moderately doped the semiconductor in which there is an impurity band separated by a forbidden region from an “ intrinsic” band in the crystal (the conduction or valence band). The energy spectrum for this situation is shown in Fig. 2 (the region corresponding to the impurity band is *This analogy is not complete because the fact that the impurity atoms are located aperiodically is ignored. Moreover, the assumption of a periodic distribution of the impurity atoms (with a period equal to a multiple of the lattice periodicity) would im ply the absence of impurity scattering, which is clearly at variance with experiment.

I M P U R I T Y L E V E L S AND I M P U R I T Y BANDS

7

Fig. 2. Moderately doped semiconductor.

crosshatched). Drawing sharp edges on the impurity band is somewhat conditional, they, too, can be smeared out. The impurity concentration at which the development of an impurity band becomes noticeable depends on the nature of the atoms and can be calculated only within the framework of some specific model. One of the methods for experimentally detecting impurity bands involves a study of the low-temperature electrical properties of the crystal. When an impurity band exists, the electrical conductivity does not become zero upon “ sweeping out” electrons from the conduction band (or holes from the valence band) but remains finite, though small (see, for exam ple, [7]). The Hall constant R also exhibits a distinctive tem perature dependence. As is easily verified, in the presence of two bands with ca rrie rs of only one type it is given by the equation [7] ec(niUj+njUj)2

Here nu pi, and n2, p2, are the concentration, drift and Hall mobility of ca rrie rs in bands 1 and 2. If the temperature dependence of the mobility is neglected, Eq. (2.1) has a maxi mum when nipi=n*|i2-

(2 . 2 )

At the same time, in the absence of an impurity band(p2=0) we would have had R~'/rii, i.e., the Hall constant would increase monotonically with a decrease in temperature.

8

ELECTRON THEORY OF SEM ICONDUCTORS

Using the above reasoning it was established that in the particular case of germanium doped with group V donors a spreading of the level becomes noticeable at an impurity con centration of n ~ 1015 cm-3.* The “width” of the impurity band obviously increases as n is increased. This can be observed experimentally as, for ex ample, a decrease in the activation energy which determines the concentration of electrons in the conduction band [8], At a sufficiently high impurity concentration the activation energy finally becomes zero. (In germanium and silicon, doped with group V donors, this occurs at n ~ 3 x 1017 cm-3andrc ~ 1018 cm-3, respectively [8, 9]). This would indicate that the upper edge of the impurity band reaches into the conduction band (Fig. 3). Under these conditions, strictly speaking, one cannot speak of an impurity band and of a conduction band literally—a single continuous spectrum emerges. We will designate as heavily doped the semiconductor in which the impurity band overlaps the intrinsic band next to it.

Fig. 3. Heavily doped n-type semiconductor.

The first important characteristic of heavily (and moderately) doped semiconductors follows directly from the definition: the impurity simultaneously shapes the characteristics of the charge c a rrie r spectrum and causes their scattering. We note that in the opposite case of light doping the electrons localized at the *Here we are not concerned with the question of the conduction mechanism in terms of the impurity band. It can vary, depending, in particular, on the mechansism by which the band is formed. For our purposes it is sufficient to bear in mind that any factor that provides a possibility for direct electron transitions between impurity atoms also leads simultaneously to a broadening of the level.

I M P U R I T Y L E V E L S AND I M P U R I T Y BANDS

9

impurity levels do not take part in the migration process, and the structure of the conduction band is practically independent of the presence of impurities. In other words, in the case of low impurity concentration the impurity atoms shape only the spectrum of the bound charge ca rrie rs and cause scattering of the free ca rrie rs with practically no change in the la tte rs’ energy spectrum. In the case of heavy and moderate doping the impurity plays both roles simultaneously. A second characteristic of heavily doped semiconductors is also evident: in the absence of compensation a degeneracy of the electron gas, even though partial, should be expected.* *Here and in analogous ca ses later on, we will consider the material to be n-type for definiteness. All considerations carry over to the case of holes by a simple change of words and symbols.

CHAPTER 3

N e u t r a l i z a t i o n in T e r m s o f Im p urit y Configurations.

Crystal M o m e n t u m

A third characteristic of heavily (and moderately) doped semiconductors can be exposed by noting that most of the elec tronic characteristics of the system that are directly calculated from quantum mechanics depend on the arrangement of the im purity atoms. The reason for this is obvious: in the solution of the appropriate dynamic problem the coordinates of the impurity atoms can mostly be assumed to be formally given because they also enter the answer as param eters.* On the other hand, the actual coordinates of the impurity atoms are certainly not given in an experiment and the “ answer,” containing so many unknown param eters (~ 1018, for example) is of no interest. It should also be remembered that in different parts of the crystal the impurity can be distributed differently, whereas the result of a macroscopic experiment refers to the entire crystal and not to individual small portions of it. In other words, an averaging of the desired quantities over the entire volume of the crystal occurs in the macroscopic experiment. The third important characteristic of heavily (and moderately) doped semiconductors consists of the requirement of this averaging. Let the total number of impurity atoms in the crystal be N, and their radius vectors be Let us designate by *ln the case of light doping one can solve the dynamic problem concerning the be havior of electrons in the presence of only one impurity atom and then “multiply the resulting value” by n. For this reason the question of the location of the impurity does not appear—one can simply assume that the given impurity atom is located at the origin of the coordinates.

11

12

ELECTRON THEORY OF SEMICONDUCTORS

P(Ri,..„ i...c?Ry the probability that atom 1 is located in the volume element dR\ about the point R,, atom 2 in the volume element dRz about the point R.2 , etc. Then the average value (over the impurity configurations) of any physical quantity A(Ri, R^ is defined by A=

(Rlt..., Ry) P(Ri, . . . , R N)dRi... dRN,

(3.1)

where the integral is over the entire volume £1 of the crystal. Obviously the normalization condition P (Ri....» Ry) dRi... dRw= 1

(3.2)

must be imposed. In what follows (with the exception of Chap. 15) we will as sume that the impurity atoms are arranged uniformly on the average, in the lattice. This means that integrals of the type in Eq. (3.1) are not taken over the entire volume of the crystal but only over some relatively large portion of it that is independent of the location of this portion in the lattice. A lattice for which this method is valid is said to be macroscopically homogeneous. Its symmetry is obviously the symmetry of the corresponding ideal lattice. This circumstance allows one to introduce the concept of the crystal momentum of the charge ca rrie r. Of course, because of the translational symmetry of the lattice the one-particle density matrix, p(r, r'), has the following properties: P(r, r') = p (r + a, r') = p(r, r' + a), (3.3) where a is a lattice vector. Consequently, the eigenfunctions of p(r, r') are Bloch functions, characterized in particular by the crystal momentum p (see [10]). The equation for these eigen functions in the coordinate representation has the form ^ P(r>Ot|) (r')dr’=

(r),

(3.4)

where g are the eigenvalues. Making the substitution r -+ r+ a and bearing Eq. (3.3) in mind, we see that the function ^(r-i-a) satis fies the same equation with the same boundary conditions. The eigenvalues g, are obviously characterized by the crystal mo mentum p and the “band index” I; as is known, in a system of Ferm i particles they are equal to zero or unity. It is simple to verify this by employing the well-known representation of p (r, r') in term s of the particle creation and annihilation operators a and a ([11, 12]):

NEUTRALIZATION

IN T E R M S O F I M P U R I T Y C O N F I G U R A T I O N S

P(r> r')= = 2 p, p'

2 (P.

1.r

0 < * 'i '< b i > f

(3 *7)

where (p, / 1j | p', /') are the matrix elements of the current-density operator in a system of Bloch functions, and the index “ f” on the average symbol means that one must perform the averaging operation while taking account of external electric and magnetic fields. The single particle density, ( a p-i-api')! , generally speak ing, is not diagonal in the (p, /) representation. In weak electric fields, however, it can be expanded in a series in term s of the field intensity [12]; then Eq. (3.7) (in the absence of a magnetic field) ultimately assumes the obvious form = 2 ( P . / | J | P .

(3 ./)

P. I

where nf (p, /) is the average number of particles in the state (p, /), calculated while taking account of the external fields. Equation (3.7/) justifies the name “ charge c a rrie rs” (or free

14

ELECTRON THEORY OF SEMICONDUCTORS

charge carriers) frequently given to particles in states of given crystal moments. An equation like (3.7) is also valid for any other additive physical quantity. Let its corresponding operator be 4. In the absence of external fields the exact formula is clearly emt. (5.22)

Here m is a quantity with dimensions of mass (sometimes called the inertial effective mass) for which an explicit expression can be found (e.g., in [12]) (see also Chap. 12); yp(0) is the Heisenberg velocity operator for t = 0. Sometimes a somewhat different form of Eq. (5.21) is con venient. That is, by noting that fVO dt

^ dx'/p (x', 0>

C H A R A C T E R IS T IC S OF A M A N Y -E L E C T R O N S Y S T E M

31

we obtain from Eq. (5.21) +00

i

crap(0) = ]im —- $ dt%{t)ehEt §dx'([/a(x, t), /p(x', 0)]_>. (5.23) — CO

In a spatially homogeneous system the correlation function of the currents,

(6.3)

(the function (5.10) is its own Fourier transform with respect to coordinates in a spatially homogeneous system). Employing Eqs. (6.1) and (6.2) we find 'df + £ ; Vv - ^ (x) -

u 0

(x)} Gr (X, x'; t —n -

— Cdx"Fc(x —x") Gv (x", x", x, t \ x', t')= - h b { x — x')b{t-t'). J (6.4) Here G2r is the second Green’s function: Gv (x", x", x, t\ x\ t')=iQ(t—( ' ) ( [a(x'', t)a(x", t)a(x, t),

a(x',r)]+>

(6.5)

Differentiating Gr(x, x'\ t—t') with respect to t', we obtain in an analogous manner an equation sim ilar to Eq. (6.4). As the boundary conditions for this equation one may take the usual periodic boundary conditions within a cube of volume Q. These conditions will generally not play a role when the specimen is sufficiently large and we are not interested in surface effects. The initial condition (i.e., the boundary condition with respect to the variable t — t'), according to Eq. (6.3), has the form Gr (x, x'; f—0 = 0

( /_ /'< 0 ) . (6.6)

The effect of the screening of the external field by the free charges, as well as all other effects of the interaction between electrons, is contained in the last term on the left side of

35

EQ U A TIO N S FO R G R EEN FU N C T IO N S

Eq. (6.4). It is obviously convenient to isolate the terras respon sible for this effect by changing over from the unscreened potential t/0(x) to the screened potential U(x). To this end we note that in a system of particles with Coulombic interaction the potential energy of an electron in the screened field of the defects, U(x), satisfies the Poisson equation (in Gaussian units): vW (x) = ~ ~ {p*4x)-f AP;(x)}.

(6.7)

6

Here pt is the space-charge density of the structural defects. If the motion of the impurity atoms is neglected, pt is independent of U. The functional Ap' [t/] is the variation of the charge density of all electrons except the given one in the field of the impurity atoms. An explicit expression for A p'e accurate to term s of any order of U can be derived by using (e.g.,) the method of [44], We re stric t ourselves to a linear approximation (which, in the classical region, corresponds to the Debye approximation). Then, according to [12], (6